# a single-layer wide-angle negative-index metamaterial at visible frequencies

TRANSCRIPT

LETTERSPUBLISHED ONLINE: 18 APRIL 2010 | DOI: 10.1038/NMAT2747

A single-layer wide-angle negative-indexmetamaterial at visible frequenciesStanley P. Burgos1†, Rene deWaele2†, Albert Polman2 and Harry A. Atwater1*Metamaterials are materials with artificial electromagneticproperties defined by their sub-wavelength structure ratherthan their chemical composition. Negative-index materials(NIMs) are a special class of metamaterials characterizedby an effective negative index that gives rise to suchunusual wave behaviour as backwards phase propagation andnegative refraction. These extraordinary properties lead tomany interesting functions such as sub-diffraction imaging1,2

and invisibility cloaking3–6. So far, NIMs have been realizedthrough layering of resonant structures, such as split-ringresonators, and have been demonstrated at microwave7,8 toinfrared9–13 frequencies over a narrow range of angles-of-incidence and polarization. However, resonant-element NIMdesigns suffer from the limitations of not being scalable tooperate at visible frequencies because of intrinsic fabricationlimitations14, require multiple functional layers to achievestrong scattering13,14 and have refractive indices that arehighly dependent on angle of incidence and polarization.Here we report a metamaterial composed of a single layerof coupled plasmonic coaxial waveguides that exhibits aneffective refractive index of−2 in the blue spectral region witha figure-of-merit larger than 8. The resulting NIM refractiveindex is insensitive to both polarization and angle-of-incidenceover a ±50◦ angular range, yielding a wide-angle NIM atvisible frequencies.

Negative-index materials were first predicted theoretically byVeselago15 in 1968, but it was only a decade ago that Pendry16defined NIM designs suitable for experimental realization. Inthese resonant-element based NIMs, the unusual ‘left handed’behaviour of light originates from subwavelength resonant elementsthat behave like ‘artificial atoms’ with engineered diamagneticresonances that are the source of the material’s negative-indexresponse. As such, NIMs were first demonstrated experimentallywith arrays ofmillimetre-size copper strips and split-ring resonatorsoperating at microwave frequencies16,17. This discovery sparked aconsiderable effort to scale down the size of the constituent resonantcomponents to enable operation at higher frequencies. As a result,micrometre-size structures have been successfully fabricated toproduce negative refractive indices at terahertz frequencies. Morerecently, NIMs have been fabricated to operate in the near-infraredspectral region. However, for operation at optical frequencies therequired size of sub wavelength scatterers is very close to practicalfabrication limits. So far, the highest reported operational frequencyof NIMs has been demonstrated at the deep-red side of the visiblespectrum (λ0 = 780 nm) using ‘fishnet’ structures with features assmall as 8 nm (ref. 14). Moreover, to achieve strong scattering, thematerial was built up from a stack of multiple physical layers—thuscomplicating the fabrication of resonant-element based NIMs foroperation at visible frequencies.

1Kavli Nanoscience Institute, California Institute of Technology, MS 128-95, Pasadena, California 91125, USA, 2Center for Nanophotonics, FOM InstituteAMOLF, Science Park 104, 1098 XG Amsterdam, The Netherlands. †These authors contributed equally to this work. *e-mail: [email protected].

Recently, using waveguides, a conceptually different approachwas taken to achieve a negative refractive index in the optical spec-tral range. Investigation of the mode structure of two-dimensionalmetal/insulator/metal (MIM) plasmonic slab waveguides18,19 re-veals that certain MIM waveguide geometries support negative-index modes at visible frequencies. Arrays of such negative-indexMIM slab waveguides can serve as a quasi three-dimensionalmetamaterial20. However, the negative-index mode in MIMwaveguides18 can only be excited from free space with the perpen-dicular polarization and off-normal angles of incidence because ofthe polarization and symmetry of themode, respectively.

These practical limitations of planar MIM geometries can becircumvented in a coaxial MIM geometry in which the planarMIM waveguide is wrapped onto itself (Fig. 1). Similar to themodes supported by planar MIM plasmonic waveguides, thecoaxial waveguide geometry is found to also support field sym-metric and anti-symmetric modes that correspond to positive-and negative-index modes, respectively. However, unlike planarMIM waveguides, calculations of individual MIM plasmonic coax-ial waveguides show a negative-index mode that, owing to thecylindrical symmetry of the structure, is accessible from freespace independent of both incidence angle and polarization. Here,we demonstrate that a two-dimensional array of vertically ori-ented MIM coaxial waveguides, arranged in a dense hexago-nal configuration, functions as a single-layer wide-angle nega-tive index material down to the blue part of the visible spec-trum. Through parameter retrieval analysis, we verify the NIM tohave a double-negative21 index band in the 450–500 nm spectralrange. Furthermore, we find that the effective refractive indexof this geometry is insensitive to both polarization and angleof incidence up to ±50◦. Unlike the wire arrays of Liu et al.,which exhibit negative refraction but not a negative index22, thecoupled coaxial waveguide array exhibits a true negative refrac-tive index characterized by negative refraction and backwardsphase propagation.

Figure 1a schematically depicts the NIM, consisting of a hexago-nal close-packed array of Ag/GaP/AgMIMcoaxial waveguides com-posed of 25 nm GaP annular channels with a 75 nm inner diameterset at a pitch of p = 165 nm in a Ag layer. We study the meta-material response both by analytic waveguide modal analysis forsingle coaxial structures, and using finite-difference time-domain(FDTD) simulations for the array of coupled coaxial waveguides.

To estimate the effective refractive index of the material,we first calculate the mode index dispersion of the constituentcoaxial elements by solving Maxwell’s equations in cylindricalcoordinates23,24 for a single MIM coaxial waveguide of infinitelength. The waveguide eigenmodes are characterized by a complexpropagation constant along the z axis β(ω)=β ′(ω)+iβ ′′(ω), whereβ ′ and β ′′ are the real and imaginary parts of the propagation

NATUREMATERIALS | ADVANCE ONLINE PUBLICATION | www.nature.com/naturematerials 1© 2010 Macmillan Publishers Limited. All rights reserved.

LETTERS NATURE MATERIALS DOI: 10.1038/NMAT2747

p-pol

s-polθx

yz

r2 r1

k

a b

p

Figure 1 |Negative-index metamaterial geometry. a, Single-layer NIM slab consisting of a hexagonal array of subwavelength coaxial waveguidestructures. The inner radius r1, outer radius r2 and array pitch p are defined in the image. b, Unit cell of the periodic structure. The angle-of-incidence θ isshown, as well as the in-plane (p-) and out-of-plane (s-) polarization directions associated with the incident wavevector k.

¬0.2 0 0.2 0.4

a b c d

827

620

496

413

650 nm

483 nm

FOM

Ener

gy (

eV) 11.4

541

x

y

x

y

′ (nm¬1)

1.5

2.0

2.5

3.0

2.3ω

′′ (nm¬1) Mode index (nmode)

Freespace wavelength 0 (nm

)

SP

β β

λ

10¬4 10¬3 10¬2 10¬1 100 ¬20 ¬10 0 10 20 30 40 101100 10210¬2 10¬1

Figure 2 | Coaxial waveguide dispersion relations. The coaxial waveguide consists of an infinitely long 25 nm GaP annular channel with a 75 nm innerdiameter embedded in Ag. Plotted are the two lowest order linearly polarized modes that most strongly couple to free space radiation. a–c, Energy isplotted versus β ′ (a), β ′′ (b) and mode index nmode (c). d, The figure-of-merit FOM= |β ′/β ′′|. The Ag/GaP planar surface plasmon energy ath̄ωSP= 2.3 eV (λ0= 540 nm) is indicated by the black dashed horizontal line. All panels show one mode with positive index (red curve) and one modewith a negative index (blue curve) below an energy of 2.7 eV (λ0=460 nm). The insets in a show the Re(Hy) (out-of-page) field distribution in thewaveguide at a wavelength of λ0=650 nm for the positive-index mode and at λ0=483 nm for the negative-index mode.

constant, respectively. Complex optical constants for Ag (ref. 25)andGaP (ref. 26) are taken from tabulated literature data.

Figure 2a and b show the calculated dispersion relationsω(β ′) and ω(β ′′) of a single Ag/GaP/Ag coaxial waveguide. Themode index nmode = cβ ′/ω is plotted in Fig. 2c. Similar to whatis reported for planar MIM structures18 we find one mode witha positive index over the entire spectral range (red curve), and asecond mode with a negative index for energies below 2.7 eV (bluecurve). The index of the second mode ranges from −9< nmode< 1in the energy range of Fig. 2. The insets in Fig. 2a show theRe(Hy) field profiles corresponding to the positive-index mode atλ0 = 650 nm (nmode = 8.5) and the negative-index mode at λ0 =483 nm (nmode=−2.0). A full field map of the negative-index modecan be found in Supplementary Fig. S1. Figure 2b shows that forenergies below h̄ωSP = 2.3 eV the positive-index mode (red curve)has the lowest attenuation and will therefore be dominant, whereasfor energies above h̄ωSP the negative-index mode (blue curve) isdominant. Figure 2d shows the figure-of-merit, FOM = |β ′/β ′′|(ref. 27), of the two modes. The lowest attenuation constant β ′′for the negative-index mode is found at λ0 = 483 nm, with acorresponding FOM of 8.3.

Next, we analyse the collective response of the coupled coaxialwaveguide array using the FDTD method. Figure 3a shows a time-snapshot of Re(Hy) inside a 165 nm pitch coaxial waveguide arrayilluminated by a λ0 = 483 nm p-polarized plane wave incidentat 30◦. At this pitch the waveguides are separated by 40 nm,corresponding to twice the radial skin depth (δ ∼ 20 nm) of anisolated coaxial waveguide mode into the Ag cladding. Phase frontsare observed to clearly refract in the negative direction, that is,

to the same side of the interface normal. By following the phasefronts in time (Supplementary Movie S1) we observe backwardphase propagation at an angle of−12.5◦ with respect to the interfacenormal, as indicated in Fig. 3a by the blue arrow labelled k.

Using Snell’s law and the wavevector refraction angle inside thematerial, we find that the metamaterial has an effective refractiveindex of neff=−2.3, close to themode index found for an individualcoaxial waveguide at this wavelength (nmode=−2.0). Furthermore,the direction of energy flow S inside the NIM layer, depictedby the green arrow in Fig. 3a, is found to be antiparallel to thephase velocity—a signature of a true negative index material.Thus, at a separation of 40 nm, the waveguides are coupled justenough to allow both power and phase to refract negatively acrossthe waveguide structures with antiparallel directions, while onlyperturbing the metamaterial’s effective index from that of a singlecoax by 1n = −0.3. From the wavelength in the metamaterialand the exponential energy decay in the waveguides we finda metamaterial FOM of 8, equal to the FOM calculated forisolated coaxial structures.

By repeating this analysis for angles ranging from 10◦ to 50◦,for both s- and p-polarized light at λ0 = 483 nm, we find verysimilar results for the material’s response, with neff varying between−2.1 and −2.4. The data for p-polarized light are summarizedin Supplementary Fig. S2. Such a small dependence of the indexon polarization and angle-of-incidence has not been demonstratedin any other NIM reported so far. For example, Valentine et al.investigated only normal incidence excitation for aNIMoperationalin the near-infrared spectral region12, whereas the negative-indexmode in planar MIM structures can only be excited at off-normal

2 NATUREMATERIALS | ADVANCE ONLINE PUBLICATION | www.nature.com/naturematerials

© 2010 Macmillan Publishers Limited. All rights reserved.

NATURE MATERIALS DOI: 10.1038/NMAT2747 LETTERS

n = 1

30°

500 nm

S k

¬12.5°

Re(Hy )

1

1

2

0 2

S0

SNIM

k0

kNIMSNIM

kNIM

bk0

p = 165 nm

Max

Min

a

neff = ¬2.14

kx /|k0|

kz /|k0|

Figure 3 |Metamaterial index. a, Light at λ0=483 nm is incident on a semi-infinite slab of single-layer negative index metamaterial at an angle of 30◦

from air. Shown is a time-snapshot of the magnetic field distribution Re(Hy) taken along the polarization plane. Arrows denote the direction of energy flowS and phase velocity k. The coax centre-to-centre pitch is schematically indicated. b, Constant-frequency surface plot at λ0=483 nm showing the relationbetween kx and kz for a semi-infinite metamaterial slab over a 50◦ range of incidence angles. The wavevector k and Poynting vector S data are derivedfrom FDTD simulations.

z eff

n eff

¬1.5

¬1.0

¬0.5

0

0.5

1.0

1.5

z’eff

z”eff

n’eff

n”eff

c d

a b

Freespace wavelength 0 (nm)480400 420 440 460 500

eff

eff

¬6

¬4

¬2

0

2

’eff

”eff

’eff

”eff

400 420 440 460 480 500

¬4

¬3

¬2

¬1

0

1

2

400 420 440 460 480 500

¬6

¬4

¬2

0

2

4

6

400 420 440 460 480 500

λ Freespace wavelength 0 (nm)λ

Freespace wavelength 0 (nm)λFreespace wavelength 0 (nm)λ

ε

ε

ε

μ

μμ

Figure 4 |NIM effective parameters. Effective parameters are calculated for a 100-nm-thick NIM slab excited at normal incidence over the 400–500 nmspectral range. a–d, The real (′) and imaginary (′′) parts of the retrieved effective relative impedance zeff (a), index neff (b), relative permittivity εeff (c) andrelative permeability µeff (d).

incidence angles and at a specific polarization18. We note thatsimulations as in Fig. 3a show the semi-infinite NIM slab to reflect∼35% of the incident light, depending on angle, indicating that asignificant fraction of light is coupled into the NIM layer. Notably,for oblique incidence, in addition to exciting the lowest orderlinearly polarized coaxial waveguide modes (n= 1), we also excitea minor contribution from the radially polarized mode (n = 0).However, this small modal overlap does not significantly changethe material index response, as both modes have similar dispersionrelations around the operation wavelength of λ0= 483 nm. Furtherdetails regarding the modal decomposition can be found in theSupplemental Information.

To further investigate the effect of coupling between coaxialwaveguides, we also performed calculations for which the pitchis set to p = 330 nm, corresponding to a waveguide separationof ∼10 skin depths. As expected, we find that for the sameexcitation conditions of λ0 = 483 nm light incident at 30◦,the waveguides are effectively decoupled with power flowingstraight down the coaxial waveguides. Indeed, by calculatingthe average Poynting vector inside the layer, we establish thatno net horizontal power flow occurs for this configuration.Thus, in the limiting case of completely decoupled waveguides,we obtain a uniaxial anisotropic medium with power flowingstraight down the one-dimensional waveguides, irrespective of

NATUREMATERIALS | ADVANCE ONLINE PUBLICATION | www.nature.com/naturematerials 3© 2010 Macmillan Publishers Limited. All rights reserved.

LETTERS NATURE MATERIALS DOI: 10.1038/NMAT2747

10 20 30 40

10 20 30 40

¬6°

500 nm

3°

Max0

b

dc

fe

|E|2

10 20 30 40

30°

¬38°

+23°

Re(Hx)

0 = 483 nm

MaxMin 0

a

λ

0 = 483 nmλ

0 = 650 nmλ

Figure 5 |Wedge refraction. a–f, A∼300-nm-thick metamaterial slab is illuminated from the left at normal (a,b,e,f) and 30◦ off-normal incidence (c,d).The right side of the slab is cut at a 3◦ angle to allow refraction (black dashed line indicates the surface normal). The wavelength of incident light is 483 nm(a–d) and 650 nm (e,f). The three panels on the left (a,c,e) depict the calculated power flow (green arrows), and the three corresponding right-side panels(b,d,f) show the steady-state electric field intensity in a polar plot, monitored at a distance of 10 µm behind the exit side of the slab. The output planesurface normal is indicated on the polar plots by a grey dot. In a we also plot the Re(Hx) field distribution along the plane of refraction.

angle of incidence. In that case, we cannot assign an effectivematerials index in terms of either power or phase, but ratherassign a local effective mode index that is characteristic of anisolated waveguide mode.

However, as the array pitch is decreased, the waveguides beginto couple in such a way that both power and phase are able topropagate across the waveguide array. We find that coupling iseasily achieved for the negative-index mode, because its stronglydelocalized field distribution, which resides primarily in the metal,allows neighbouring structures to easily couple (see Fig. 2a insetsand Supplementary Fig. S1). At a waveguide separation of roughly

twice the mode skin depth of a single coaxial waveguide modeinto the surrounding Ag, we find not only that power andphase are antiparallel, but also that they refract with an effectiveindex close to the mode index of the constituent waveguides(Supplementary Fig. S3). By varying the incidence angle, the arrayresponse is found to be isotropic within a ±50◦ angular range(Supplementary Fig. S2).

This level of isotropy can be observed in Fig. 3b, which showsthe constant-frequency surface formed by the wavevector k andPoynting vector S data derived from FDTD simulations. The figureclearly illustrates that both phase and power are antiparallel within

4 NATUREMATERIALS | ADVANCE ONLINE PUBLICATION | www.nature.com/naturematerials

© 2010 Macmillan Publishers Limited. All rights reserved.

NATURE MATERIALS DOI: 10.1038/NMAT2747 LETTERSa±50◦ range of incidence angles (corresponding to a±20◦ angularrange inside the material).

To confirm the validity of assigning an effective index to thecoupled coaxial waveguide structure, we used FDTD to performa parameter retrieval procedure28,29 on a 100-nm-thick NIM slab(Fig. 1a) over the 400–500 nm spectral range. Figure 4 shows theresulting curves corresponding to the effective relative impedancezeff, index neff, relative permittivity εeff, and relative permeabilityµeffof the coupled coaxial NIM structure, with (′) and (′′) denoting theparameters’ real and imaginary parts, respectively. The extractedeffective index curve (Fig. 4b) is found to closely resemble themodeindex dispersion of a single coaxial waveguide structure (Fig. 2c)with n′eff going from positive to negative values at λ0 ∼ 420 nm,with increasing wavelength. At λ0 = 483 nm, we obtain a retrievedeffective index of neff =−2.1+ i0.2, corresponding to a FOM∼ 10that is consistent with the single coaxial waveguide FOM ∼ 8.For the retrieved effective relative permittivity εeff (Fig. 4c) weobserve a material with ε′eff < 0 over the entire simulated spectralregion, whereas for the effective relative permeability µeff (Fig. 4d)we get a material that is diamagnetic with µ′eff < 0 over the450–500 nm spectral range. Thus, we confirm that the coupledcoaxial waveguide NIM structure has a double-negative index21composed of simultaneously negative real parts of the permittivityand permeability over the 450–500 nm spectral range.

To further corroborate our results, we have simulated theSnell–Descartes refraction of a ∼300-nm-thick wedged-shapedmetamaterial slab cut at a 3◦ angle. Figure 5a depicts a time snapshotof the steady state Re(Hx) field distribution along the plane ofrefraction for λ0 = 483 nm s-polarized light at normal incidence(Supplementary Movie S2). Figure 5a shows that light refractsnegatively at the angled side of the prism, exiting the structureat an angle of −6◦ with respect to the surface normal. Figure 5bshows a polar plot of the refracted light projected into the far field.Using Snell’s law and the observed negative refraction angle, wederive a refractive index for the metamaterial slab of neff =−1.8,in agreement with the effective index derived from the observedwavevector inside the semi-infinite slab.

To demonstrate the insensitivity of the metamaterial-index toincidence angle, we also simulated the refraction of off-normalincident light through the 3◦ wedge. Figure 5c and d show thesimulation results for λ0 = 483 nm radiation incident at 30◦. Thegreen arrows in Fig. 5c indicate the direction of the Poynting vectorfor the incident and refracted beams. In this case the beam isrefracted at an angle of −38◦ with respect to the surface normal,corresponding to an effective index neff =−2.2, again consistentwith the effective index found for the wedge excited at normalincidence. By varying the angle-of-incidence fromnormal incidenceup to 50◦ for both s- and p-polarized light, we find consistentrefractive indices ranging from −1.8 to −2.4. These data aresummarized in Supplementary Fig. S2.

To illustrate the metamaterial’s tunability with wavelength, westudy the refraction of λ0 = 650 nm radiation for which the modeindex dispersion of a single waveguide element (Fig. 2a) shows apositive index (nmode = 8.5). Indeed, as Fig. 5e and f show, thebeam is now refracted to the opposite side of the interface normal,at an angle of 23◦, corresponding to a positive effective index ofneff = 7.4. We attribute the difference between the metamaterialeffective index and isolated waveguide mode index to the possibleexcitation of higher-order waveguide modes. Thus, by illuminatingthe structure with frequencies either above or below the Ag/GaPsurface plasmon resonance, we can excite both positive and negativerefractive indices within the samemetamaterial.

Realization of the metamaterial structure reported here involvesthe challenge of fabricating high-aspect-ratio nanoscale Ag chan-nels. However, we have shown that 50-nm-wide coaxial apertureswith aspect ratios >10 can readily be fabricated using focused

ion beam milling30. For large-scale fabrication, a more tractableapproach would be to use electron beam lithography in combi-nation with high aspect ratio reactive ion etching. We also notethat observation of the negative-index response requires only amodest total material thickness, that is, thick enough for a singlewaveguide to support the negative index waveguidemode. This can,for instance, be seen in our wedge simulations (for example, Fig. 5a)where the wedge thickness is only ∼300 nm and the material’snegative index response is clearly observed. At λ0 = 483 nm for anindex of n=−2, a minimum thickness of ∼120 nm is required,corresponding to amodest coaxial channel aspect ratio of 4.

MethodsCoaxial waveguide dispersion relation. The dispersion relation of the constituentcoaxial elements is calculated by solving Maxwell’s equations in cylindricalcoordinates23,24 for a single MIM coaxial waveguide of infinite length. Theazimuthal dependence of the electric and magnetic fields in the waveguide isdescribed by the harmonic function einψ of order n. We consider only the modeswith n= 1 as these are the lowest order linearly polarized modes that most stronglycouple to free space radiation. The radial dependence of the fields in all threedomains (metal–dielectric–metal) is described by solutions to the second orderBessel differential equation. We apply a Bessel function of the first kind Jn to theAg core; a Hankel function of the first kind Hn to the Ag cladding; and a linearcombination of both Jn andHn functions to the dielectric channel. On each domainboundary we formulate four continuity conditions for the tangential componentsof the electric and magnetic fields. The optical eigenmodes of the coaxial waveguideare found when the determinant of the resulting homogeneous system of eightequations with eight unknown coefficients vanishes.

NIM slab refraction. For the semi-infinite metamaterial slab calculations, the NIMis modelled in FDTD (Lumerical FDTD Solutions 6.0) as a single unit cell (Fig. 1b)embedded in air with Bloch boundary conditions along the in-plane direction. Thestructure is excited with a continuous plane wave source incident at an angle θ .The appropriate electromagnetic fields are recorded to reconstruct the refraction ofphase (Fig. 3a) along the plane of incidence. The refraction of power is obtained byspatially averaging the steady state Poynting vector components inside the materialalong the plane of incidence. The steady state electromagnetic fields are obtained bycalculating the system’s impulse response to a plane wave source with a Gaussianfrequency spectrum centred at the frequency of interest.

Parameter retrieval. The parameter retrieval is calculated using FDTD by excitinga 100-nm-thick NIM slab embedded in air with a broadband plane wave sourceranging from λ0 = 400 to 500 nm at normal incidence. The steady state fielddistributions are recorded, and the complex reflection r and transmission tcoefficients are calculated by taking the ratios r = Er/E0 and t = Et /E0, whereE0 is the electric field amplitude of the incident wave and Er and Et are thereflected and transmitted electric field amplitudes, respectively. Standard invertedreflection and transmission parameter equations found in literature28,29 areused to relate r and t to the layer’s effective impedance zeff and index neff. Theeffective permittivity εeff and permeability µeff are calculated through the relationsε= n/z and µ= nz .

Wedge refraction. For the wedge refraction simulations, the NIM wedge ismodelled in FDTD as a ∼300-nm-thick metamaterial-slab cut at a 3◦ angle.The structure is excited with a continuous wave source centred at the desiredexcitation frequency using a ∼1-µm-wide hollow metallic waveguide orientedperpendicular to the metamaterial’s input plane. The appropriate electromagneticfields are recorded to reconstruct the refraction of phase (Fig. 5a) along the planeof incidence. The structure is also excited from free space with a ∼1.5 µm spotsize Gaussian beam. Using the steady state field distribution at the output sideof the wedge, a near-to-far-field transformation is performed to determine therefracted-beamprofile at a distance of 10 µmbehind the exit side of the structure.

Received 28 October 2009; accepted 15 March 2010;published online 18 April 2010

References1. Pendry, J. B. Negative refraction makes a perfect lens. Phys. Rev. Lett. 85,

3966–3969 (2000).2. Fang, N., Lee, H., Sun, C. & Zhang, X. Sub-diffraction-limited optical imaging

with a silver superlens. Science 308, 534–537 (2005).3. Alu, A. & Engheta, N. Multifrequency optical invisibility cloak with layered

plasmonic shells. Phys. Rev. Lett. 100, 113901 (2008).4. Cai, W., Chettiar, U. K., Kildishev, A. V. & Shalaev, V. M. Optical cloaking

with metamaterials. Nature Photon. 1, 224–227 (2007).5. Liu, R. et al. Broadband ground-plane cloak. Science 323, 366–369 (2009).

NATUREMATERIALS | ADVANCE ONLINE PUBLICATION | www.nature.com/naturematerials 5© 2010 Macmillan Publishers Limited. All rights reserved.

LETTERS NATURE MATERIALS DOI: 10.1038/NMAT2747

6. Pendry, J. B., Schurig, D. & Smith, D. R. Controlling electromagnetic fields.Science 312, 1780–1782 (2006).

7. Parazzoli, C. G. et al. Experimental verification and simulation of negativeindex of refraction using Snell’s law. Phys. Rev. Lett. 90, 107401 (2003).

8. Shelby, R. A., Smith, D. R. & Schultz, S. Experimental verification of a negativeindex of refraction. Science 292, 77–79 (2001).

9. Dolling, G. et al. Simultaneous negative phase and group velocity of light in ametamaterial. Science 312, 892–894 (2006).

10. Dolling, G., Wegener, M. & Linden, S. Realization of a three-functional-layernegative-index photonic metamaterial. Opt. Lett. 32, 551–553 (2007).

11. Shalaev, V. M. et al. Negative index of refraction in optical metamaterials.Opt. Lett. 30, 3356–3358 (2005).

12. Valentine, J. et al. Three-dimensional optical metamaterial with a negativerefractive index. Nature 455, 376–379 (2008).

13. Zhang, S. et al. Experimental demonstration of near-infrared negative-indexmetamaterials. Phys. Rev. Lett. 95, 137404 (2005).

14. Dolling, G., Wegener, M., Soukoulis, C. M. & Linden, S. Negative-indexmetamaterial at 780 nm wavelength. Opt. Lett. 32, 53–55 (2007).

15. Veselago, V. G. The electrodynamics of substances with simultaneouslynegative values of ε and µ. Sov. Phys. Usp. 10, 509–514 (1968).

16. Pendry, J. B., Holden, A. J., Robbins, D. J. & Stewart, W. J. Magnetism fromconductors and enhanced nonlinear phenomena. IEEE Trans. Microw. Theory47, 2075–2084 (1999).

17. Smith, D. R. et al. Composite medium with simultaneously negativepermeability and permittivity. Phys. Rev. Lett. 84, 4184–4187 (2000).

18. Dionne, J. A., Verhagen, E., Polman, A. & Atwater, H. A. Are negative indexmaterials achievable with surface plasmon waveguides? A case study of threeplasmonic geometries. Opt. Express 16, 19001–19017 (2008).

19. Lezec, H. J., Dionne, J. A. & Atwater, H. A. Negative refraction at visiblefrequencies. Science 316, 430–432 (2007).

20. Shvets, G. Photonic approach to making a material with a negative index ofrefraction. Phys. Rev. B 67, 035109 (2003).

21. Chettiar, U. K. et al. Dual-band negative index metamaterial: Double negativeat 813 nm and single negative at 772 nm. Opt. Lett. 32, 1671–1673 (2007).

22. Liu, Y., Bartal, G. & Zhang, X. All-angle negative refraction and imaging in abulk mediummade of metallic nanowires in the visible region. Opt. Express 16,15439–15448 (2008).

23. Baida, F. I., Belkhir, A., Labeke, D. V. & Lamrous, O. Subwavelength metalliccoaxial waveguides in the optical range: Role of the plasmonic modes.Phys. Rev. B 74, 205419 (2006).

24. Novotny, L. & Hafner, C. Light propagation in a cylindrical waveguide with acomplex, metallic, dielectric function. Phys. Rev. E 50, 4094–4106 (1994).

25. Johnson, P. B. & Christy, R. W. Optical constants of the noble metals.Phys. Rev. B 6, 4370–4379 (1972).

26. Palik, E. D. & Ghosh, G. Handbook of Optical Constants of Solids(Academic, 1985).

27. Soukoulis, C. M., Linden, S. &Wegener, M. Negative refractive index at opticalwavelengths. Science 315, 47–49 (2007).

28. Smith, D. R., Vier, D. C., Koschny, T. & Soukoulis, C. M. Electromagneticparameter retrieval from inhomogeneous metamaterials. Phys. Rev. E 71,036617 (2005).

29. Minowa, Y. et al. Evaluation of effective electric permittivity and magneticpermeability in metamaterial slabs by terahertz time-domain spectroscopy.Opt. Express 16, 4785–4796 (2008).

30. de Waele, R., Burgos, S. P., Polman, A. & Atwater, H. A. Plasmon dispersionin coaxial waveguides from single-cavity optical transmission measurements.Nano Lett. 9, 2832–2837 (2009).

AcknowledgementsWe would like to thank J. A. Dionne, H. J. Lezec, E. Verhagen, and A. F. Koenderinkfor fruitful discussions. This work was supported by the Energy Frontier ResearchCenter program of the Office of Science of the Department of Energy under grantDE-SC0001293, by the National Science Foundation under the Graduate ResearchFellowship Program, and made use of facilities supported by the Center for Scienceand Engineering of Materials, an NSF Materials Research Science and EngineeringCenter at Caltech. This work is also part of the research program of the ‘Stichtingvoor Fundamenteel Onderzoek der Materie (FOM)’, which is financially supported bythe ‘Nederlandse Organisatie voor Wetenschappelijk Onderzoek (NWO)’. It was alsosupported by ‘NanoNed’, a nanotechnology program funded by the Dutch Ministryof Economic Affairs.

Author contributionsH.A.A. conceived the idea. H.A.A. and A.P. provided guidance throughout the project’sdevelopment. S.P.B. took the lead in the FDTD analysis. R.D.W. took the lead indeveloping the analytic coaxial waveguide theory and code. S.P.B., R.D.W., A.P. andH.A.A. all contributed to the writing and editing of themanuscript.

Additional informationThe authors declare no competing financial interests. Supplementary informationaccompanies this paper on www.nature.com/naturematerials. Reprints and permissionsinformation is available online at http://npg.nature.com/reprintsandpermissions.Correspondence and requests formaterials should be addressed toH.A.A.

6 NATUREMATERIALS | ADVANCE ONLINE PUBLICATION | www.nature.com/naturematerials

© 2010 Macmillan Publishers Limited. All rights reserved.